Chip-scale solar thermal electrical power generation
Chip-scale solar thermal electrical power
Molecular solar thermal energy storage is a technology based on photoswitchable
materials, which allow sunlight to be stored and released as chemical energy on
demand. Wang et al. demonstrate a molecular thermal power generation system
that stores solar energy and converts it to electric power on demand.
Zhihang Wang, Zhenhua Wu,
Zhiyu Hu, ..., Fengdan Wang,
Tao Li, Kasper Moth-Poulsen
Solar energy storage and
conversion to electrical power
generation is demonstrated
Continuous power output can be
generated from the combined
Photophysical properties of two
photoswitches are fully
ultrathin thermoelectric chip is
designed and fabricated
Wang et al., Cell Reports Physical Science 3,
March 16, 2022 ª 2022 The Author(s).
Chip-scale solar thermal
electrical power generation
Zhihang Wang,1 Zhenhua Wu,2 Zhiyu Hu,2,* Jessica Orrego-Hernández,1 Erzhen Mu,3
Zhao-Yang Zhang,4 Martyn Jevric,1 Yang Liu,2 Xuecheng Fu,5 Fengdan Wang,5 Tao Li,4,*
and Kasper Moth-Poulsen1,6,7,8,*
There is an urgent need for alternative compact technologies that can
derive and store energy from the sun, especially the large amount of
solar heat that is not effectively used for power generation. Here, we
report a combination of solution- and neat-film-based molecular solar
thermal (MOST) systems, where solar energy can be stored as chem-
ical energy and released as heat, with microfabricated thermoelectric
generators to produce electricity when solar radiation is not available.
The photophysical properties of two MOST couples are characterized
both in liquid with a catalytical cycling setup and in a phase-intercon-
vertible neat film. Their suitable photophysical properties let us
combine them individually with a microelectromechanical ultrathin
thermoelectric chip to use the stored solar energy for electrical power
generation. The generator can produce, as a proof of concept, a po-
wer output of up to 0.1 nW (power output per unit volume up to
1.3 W m 3
). Our results demonstrate that such a molecular thermal
power generation system has a high potential to store and transfer
solar power into electricity and is thus potentially independent of
From the Industrial Revolution to 2018, the global average temperature increased
C as a result of human activities and may hit 1.5
C as early as 2030, as warned
by the United Nations Intergovernmental Panel on Climate Change (IPCC).1
have been actively looking for a technology that can slow down or reduce the rise in
global temperature. As the global population increases, total worldwide energy use
from all sectors is expected to reach 21 TWy by 2040, corresponding to an increase
of 130% over 2019 levels.2
Electricity is an essential commodity in modern society,
and around 3 TW is currently used. To complicate matters, about 85% of this power
is derived from fossil fuels.3
Therefore, searching for new decarbonized energy sour-
ces to reduce greenhouse gas emissions is imminent. Nuclear energy is a low-carbon
energy source, but its installations are complex, and their thermal pollution can
potentially be serious. As the most common renewable energy at present, hydro-
power is geographically limited, while wind energy fluctuates with season or
It is noteworthy that solar energy is the most abundant energy resource on
Earth, and maximizing the use of solar power can potentially meet the intensive de-
mand for power while reducing detrimental effects to the environment.5
instance, an estimated 2.3 3 104
TWy of solar power reaches Earth each year, which
equates to only 7 h of sunlight needed to meet current annual global energy
1Department of Chemistry and Chemical
Engineering, Chalmers University of Technology,
41296 Gothenburg, Sweden
2National Key Laboratory of Science and
Technology on Micro-Nano Fabrication,
Shanghai Jiao Tong University, Shanghai 200240,
3School of Materials Science and Engineering,
Henan Polytechnic University, Jiaozuo 454003,
4Shanghai Key Laboratory of Electrical Insulation
and Thermal Aging, School of Chemistry and
Chemical Engineering, Shanghai Jiao Tong
University, Shanghai 200240, China
5Center for Advanced Electronic, Materials and
Devices (AEMD) of Shanghai Jiao Tong
University, Shanghai 200240, China
6Institute of Materials Science of Barcelona,
ICMAB-CSIC, 08193 Bellaterra, Barcelona, Spain
7Catalan Institution for Research and Advanced
Studies ICREA, Pg. Lluı́s Companys 23,
*Correspondence: firstname.lastname@example.org (Z.H.),
Cell Reports Physical Science 3, 100789, March 16, 2022 ª 2022 The Author(s).
This is an open access article under the CC BY license (http://creativecommons.org/licenses/by/4.0/).
Photovoltaic (PV) cells can directly convert solar energy into electrical power with a
maximum efficiency of around 30%, and most of the solar energy is not only lost as
heat but also contributes to deteriorating the performance.8–11
In addition, solar in-
tensity naturally varies with time and geographical location and these variations
currently limit the utilization of PV. Obviously, PV cells do not produce power during
the night. Solar thermal power plants with phase-change molten salts can generate
power for several hours after sunset; however, these plants require very large solar
concentrators and consequently can be installed only in remote areas.12,13
ously, solar actuators based on hydrogen-bonded azopolymers for electricity gener-
ation have been investigated; however, the device cannot store solar energy for later
on-demand power generation.14
Hence, in addition to the above mainstream tech-
nologies, there is an urgent need for new alternative compact technologies that can
derive and store energy from the sun, especially the large amount of solar heat that is
not effectively used for future power generation. In this paper, we demonstrate a
compact, chip-based device that allows for direct storage of solar energy as chem-
ical energy that is released in the form of heat on demand and then converted into
electrical energy in a controlled way.
To explore ways to store solar energy, we are investigating a class of materials that
can capture sunlight via reversible photochemical reactions and later release this
stored energy on demand. These materials operate in a closed cycle, and they use
photochromic chemical compounds to form the basis of molecular solar thermal
(MOST) energy storage systems.15–18
Upon exposure to sunlight, a suitable MOST
material (in the parent state) can photoisomerize to a high-energy metastable photo-
isomer that can be stored for extended periods of time. Depending on the photo-
chrome used, the back-conversion reaction releasing heat energy can be triggered
through different processes, including thermal,19,20
and photoinduced conversion.25–27
It has been previously estimated
that, for an ideal liquid MOST device, up to 21% of the solar energy can be stored
as chemical energy for later heat production.28
Such heat produced can be delivered
locally and on demand, unlike other thermal storage technologies.
While MOST systems can be used in closed-cycle devices for efficient storage and
release of heat, additional engineering is necessary to generate electrical power.
Thermoelectric generators (TEGs) are able to directly convert thermal energy into
electrical power via the Seebeck effect. TEGs have been widely used in various ap-
plications due to their attractive features such as silent operation, minimal mainte-
nance, and long lifetime. And they have been considered as promising alternatives
to meet the urgent demand for energy around the world.29,30
Traditional solar ther-
mal-to-electric power generation systems use heat engines to convert heat into elec-
tricity in two steps (heat to mechanical movements and then mechanical energy to
electrical power generation).31,32
However, a large amount of heat can be lost dur-
ing the conversion process. To solve this issue, bulk TEGs have been combined with
phase-change materials for power generation to convert heat to electricity
Recently, low-dimensional material-based microelectromechanical sys-
tem (MEMS) technology has enabled the production of ultrathin and highly sensitive
TEG devices that can integrate large arrays of thermoelectric (TE) modules.34
our previous results, we explored a reliable and efficient hybrid method for ultrathin
MEMS-TEG fabrication, and achieved up to 46,000 TE modules on a 3-in silicon
Such a MEMS-TEG equipped with an 800-nm-thin TE film has shown a
steady electrical output, which was sensitive to small temperature differences and
could effectively utilize low-grade thermal energy.37
The temperatures accessible
by the energy release reaction of the MOST are, at the current stage of
2 Cell Reports Physical Science 3, 100789, March 16, 2022
development, less than 100
C, which is not high enough to be utilized for electrical
power generation by traditional means. Therefore, it is necessary to match the
MOST systems with high-efficiency and sensitive TE devices to effectively utilize
this relatively low-grade thermal energy.
Here, we design a compact, chip-based device that combines two different MOST
systems operating either in the liquid or in the solid state with a novel designed
MEMS-TEG to demonstrate the storage of solar energy to the release of heat energy
and the cascading energy flow to the harvester that is finally used to generate power
(see Scheme 1). Two molecular photoswitches with suitable properties—a norborna-
diene derivative (NBD) investigated as a solution and a phase-interconvertible ary-
lazopyrazole derivative (AZO) measured as a neat film—are selected for their poten-
tial to produce heat energy for electrical generation. The ultrathin MEMS-TEG with
572 TE modules is designed and fabricated, in which the TE films are only 1 mm thick.
We characterize and couple each of these photoswitches individually with the
MEMS-TEG chip (effective thermoelectricity area 10 3 6 mm), demonstrating that
chemical energy stored in MOST systems (in Sweden) can successfully generate
electrical power (in China) through the process of solar energy storage, heat release,
and TE conversion, thus affirming that solar energy can generate electrical power in-
dependent of time and geographical restrictions.
RESULTS AND DISCUSSION
Solar energy storage properties
MOST systems can function in both liquid and film forms, which can be tailored toward
In liquid form, MOST systems can transport stored en-
ergy, meaning that energy can be stored and released in two different locations,
whereas in film form, MOST systems can be used in smart windows and other device
In this study, we selected and tested two systems: an NBD in
liquid form (in toluene solution, which can provide a low specific-heat capacity of ca.
1.6 J g 1
) and a neat AZO in thin films with suitable energy capture and storage
functionality. The molecular structures of both photoswitch couples are shown in Fig-
ure 1A. The photoconversion of NBD proceeds via a [2 + 2p] cycloaddition reaction
to its corresponding photoisomer quadricyclane derivative (QC). Thus, the energy stor-
age density DHstorage was experimentally determined to be 93 kJ mol 1
(0.37 MJ kg 1
Meanwhile, QC has a thermal back conversion half-life of 1 month at room temperature,
demonstrating the possibility for long-term storage in toluene. Spectroscopically, we
previously showed that norbornadiene with a push-pull system has a spectral red-shift-
ing effect on the absorption.21
Hence, this NBD with dimethoxy donor units exhibits an
absorption feature around 340 nm with a maximum absorptivity of εmax@340 nm = 1.4 3
. In contrast, the absorption profile of QC is virtually negligible above
300 nm, leaving a transparent optical window of around 85 nm between both forms
due to the selected push-pull substituents (see Figure 1B). This significant spectral
Scheme 1. Schematic illustration of the MOST to power generation concept
Cell Reports Physical Science 3, 100789, March 16, 2022 3
difference enables near-quantitative photoconversion, even in concentrated solutions.
In addition, the photoisomerization quantum yield was 68% in toluene. Considering the
above-mentioned MOST properties, solar energy storage efficiency of the system
could exceed 0.70%38
(see Note S1 for details).
Neat-film thermal storage devices have several attractive features, such as simple de-
vice integration and no need for mechanical pumping. Further, systems that combine
energy input from solar irradiation with absorption of ambient heat have recently
Such systems couple a phase-change event to the photoconversion
process found in MOST systems. One example is the AZO explored here (see Fig-
ure 1A). To take advantage of the exothermic process not only from the photoisome-
rization reaction but also from an additional phase-change process (liquid / crystal),
we investigated the AZO photoswitch in its neat form. The energy stored in cis-AZO
was easily released by triggering heat release following irradiation with a 532-nm
light source (this wavelength is considered cis-AZO’s onset of absorption). As shown
in Figure 1C, the absorption maximum of the trans isomer was 344 nm with an absorp-
tivity of εmax@340 nm = 2.9 3 104
. The trans-AZO has a quantum yield of only
41%, but this is considered high for other azobenzene-based photoswitches. The
photoisomerization energy density DHisom was 52 kJ mol 1
(0.17 MJ kg 1
addition to heat release from the chemical reaction, the crystal-to-liquid transition
(DHphase_change) can provide an additional 50 kJ mol 1
(0.16 MJ kg 1
) of thermal en-
ergy because of its long alkenyl chain. As a result, the solar energy storage efficiency
of the AZO couple was estimated to be 1.2%, which is much higher than that of other
Moreover, cis-AZO is remarkably stable at room
Figure 1. Structures and absorption spectra of the two MOST candidates used in this work
(A) Molecular structures of NBD-QC couple (top) and trans/cis-AZO photoswitch couple (bottom).
A thermal (D) or catalytic (cat.) route can facilitate the back conversion of QC / NBD. The back
conversion of cis- / trans-AZO can be achieved by a thermal or light-induced activation.
(B) Absorption profile of NBD before and after irradiation with 340-nm light (in toluene).
(C) Absorption profile of AZO photoswitch before and after irradiation with 365-nm light (in
4 Cell Reports Physical Science 3, 100789, March 16, 2022
temperature, with a thermal half-life of 3 months at 25
C. Thus, using this photoswitch
from a neat film would allow two different sources of stored energy to be used: ther-
mal ambient energy and light.46,47
Photoconversion in the device under various exposure times and complete intercon-
version through multiple cycles are important tests for photoswitch viability in a
MOST system. These experimental factors have previously been reported for
but not for NBD. Therefore, additional experiments were necessary to deter-
mine the compatibility of the NBD photoswitch. A custom-made 400-mm2
dic reactor was used for this photoconversion experiment (see Note S2 and Figure S1
for details). A solution of 0.1 M NBD (25 g L 1
) in toluene-d8 was pumped through
the microfluidic reactor with residence times from 34 to 343 s. The degree of photo-
conversion was monitored immediately afterward by 1
H NMR spectroscopy. For an
ideal MOST system, where the absorption of the photoisomer (QC) does not
compete with the absorption of the parent (NBD), the energy storage efficiency,
hMOST, should remain approximately unchanged prior to full conversion.40,45,56
Here, we observed a decrease in solar energy storage efficiency from z0.5% at short
residence times to 0.25% at full conversion. While not ideal, it is normal for efficiency
to lower progressively during the conversion process. In this context, this system is
better than our previous attempts at flow conversion (see Figure 2A and Note S3 for
Typically, for cyclability testing, solution-based photoswitches are irradiated at
However, this method seemed impractical as QC has
a long half-life (t1/2z29 days) in toluene. To address this, an alternate protocol
was employed, which hastened the time frame for each successive cycle. Cobalt(II)
phthalocyanine is physisorbed on activated carbon (CoPc@C) and can rapidly facil-
itate the back reaction of a very similar quadricyclane structure.21
This new setup
involved converting and back converting an NBD solution (0.5 mM in toluene)
continuously through a microfluidic photoreactor and a catalytic reactor in a closed
Figure 2. Conversion performance, cycling performance, and experimental setup of NBD in the device
(A) Conversion percentage (in blue) and calculated energy storage efficiency (in red) of 0.1 M NBD in toluene as a function of residence time in the
(B) Normalized absorbance before irradiation with 340 nm LED light and after catalytic reactor. Blue dots show the normalized absorbance at 340 nm,
red dots show the normalized absorbance after irradiation.
(C) Cycling test setup for NBD. Boxes 1 and 2 represent the flow UV-vis spectrometer before and after a catalytic reaction center. Box 3 refers to the
microfluidic chip. The conversion process has proceeded with irradiation from a 340 nm LED lamp.
Cell Reports Physical Science 3, 100789, March 16, 2022 5
cycle. Happily, no obvious drop in performance was observed after 54 charge and
discharge cycles on the NBD couple (see Figures 2B and 2C and Note S4 for details).
This setup drastically reduced the total experimental time to only 61 h.
Stored energy release for NBD and AZO
Once solar energy is stored as QC and cis-AZO, one should be able to release the chem-
ical energy from these metastable compounds as heat. However, we performed simula-
tions to determine how much energy could be extracted from these charged materials.
To achieve this, a simulation of possible temperature increases based on molecular pa-
rameters was performed. In the case of QC, the maximum temperature increase de-
pended on the concentration of initial NBD in toluene. Based on the highest possible
concentration of 0.78 M in toluene, the maximum estimated temperature difference un-
der adiabatic conditions was 40
C (see Note S5 and Figure S2 for details).
To test the experiment in practice, we designed a fixed-bed catalytic heat-release
device consisting of a copper tube flanked on two sides with copper plates to maxi-
mize heat transfer to the MEMS-TEG device (see Note S6 and Figure S3 for details).
By taking advantage of the mobile nature of the QC solution, a heterogeneous
was loaded inside the copper tube, and a thermally conductive
pad was used to provide a homogeneous thermal distribution from the tube to all
areas of the device. A saturated NBD solution was initially photoconverted to QC
and then pumped through the reactor at a flow speed of 5 mL h 1
. This speed leads
to complete back conversion from QC to NBD and a maximum surface temperature
C maximum temperature gradient, see Figure 3A and Video S1 for de-
tails). A thermal camera recorded liquid-QC macroscopic heat release, determined
by the camera focusing on the top of the device.
Concerning the trans/cis-AZO photoswitch couple, the charged cis isomer releases
0.17 MJ kg 1
, equating to a simulated thermal difference of 84
C. From here, an
additional 0.16 MJ kg 1
can be extracted at the crystallization point of the trans-
AZO (melting point 83
C) from the phase-change event. Thus, cis-AZO theoretically
shows a larger potential thermal gradient than the QC solution. In this case,
the experimental measurement of the heat release involved the placement of a
droplet of liquid cis-AZO (z8 mg) under ambient conditions onto a glass substrate
Figure 3. Macroscopic heat-release performance of QC and cis-AZO under infrared camera
(A) Recorded temperature increment of QC heat release over time; inset shows the thermal image
from the heat-releasing copper device. The area indicated by the dashed line represents the device
(B) Recorded temperature increment of the cis-AZO system over time; inset shows the thermal
image from the heat-releasing cis-AZO sample. The dashed line represents the position of the
compound (maximum temperature gradient of 17
C after the heat generated from the laser is
6 Cell Reports Physical Science 3, 100789, March 16, 2022
(1 3 0.7 cm). A 532 nm laser was used to irradiate the sample and trigger the heat
release in conjunction with a thermal camera. This triggered a full back conversion,
affording a maximum surface temperature of 52
C, corresponding to a 17
maximum temperature difference after accounting for heat from the laser. The large
difference in temperature gradient between theoretical and experimental values is
likely due to the strong heat dissipation from the thin film under ambient conditions
(see Figure 3B and Video S2 for details). The thermal camera recorded the cis-AZO
film macroscopic heat release.
These results showed that both solution-based NBD and neat AZO photoswitches
can successfully generate heat. Next, we wanted to use this thermal energy by con-
verting it to electrical power using the MEMS-TEG device.
Single-layered microelectromechanical thermoelectric chip
Theoretically, the figures of merit (ZTave) of low-dimensional TE materials are higher
than those of bulk TE materials and can potentially yield a higher TE conversion
Thin-film-based TE devices are also sensitive to small temperature
Such technology can be used to monitor local thermal variations at
micro-nano scales, such as bioactivity in yeast cultures.58
On the other hand, if the
number of integrated TE modules is high enough, the output electrical power can
be significantly increased.59
To effectively convert the heat released from MOST
systems to electrical power, a large array integrated MEMS-TEG based on Bi2Te3
(n type) and Sb2Te3 (p type) TE modules was fabricated. The unit structure is de-
signed in a P shape, with a resistance of 72.8 U and a single p/n surface area of
200 3 200 mm. The fabrication process and structure diagram of the MEMS-TEG de-
vice are shown in Note S7, Figures S4–S9, and Table S1. In total, 572 TE modules
were connected in series, where the height of each TE column was increased to
1 mm with the aim of improving the TE performance at low temperature gradients,
Figure 4. Thermal performance of MEMS-TEG used in this work
(A) Optical microscope photo of MEMS-TEG with 572 TE modules.
(B) Three-dimensional laser scanning confocal microscope images of the fabricated thermoelectric pairs.
(C) Top view of the fabricated thermoelectric pairs by laser scanning confocal microscopy. Scale bar
shows the relative height of the device.
(D) Power generation of MEMS-TEG when hot water of different temperature flows through the
copper tube at the hot end of the TEG.
Cell Reports Physical Science 3, 100789, March 16, 2022 7
as shown in Figure 4.37
Most importantly, the thickness of the whole working part
from the chip did not exceed 2 mm. This ultrathin structure (thickness of top contact
layer of only 300 nm and a mass of only a few picograms) responded effectively to
small variations in temperature. The structure and properties of the TE materials
constituting the MEMS-TEG and the power generation performance of the device
are shown in Table S1 and Figures S5–S8. Since the heat released by QC in the cop-
per tube does not cover all the tubes uniformly, as shown in Figure 3, a reference
experiment was conducted to investigate the power generation of the MEMS-TEG
by passing hot water into the copper tube at a flow speed of 73 mL h 1
(see Figure S9). When the temperature of the inlet hot water was 36.5
C and 54.5
the corresponding voltages generated by the MEMS-TEG were 0.4 mV (maximum
power output of density 6 W m 3
) and 3 mV (maximum power output of density
349 W m 3
), respectively. This shows that the higher the average temperature in
the MOST reaction chamber, the greater the power output density can be reached.
Power generation from NBD and AZO
Based on the physical properties of NBD and AZO couples, two heat-to-power gen-
eration device concepts were put forth (see Figure 5A). For the NBD system, a satu-
rated solution of QC in toluene was prepared in Gothenburg, Sweden, using a
photochemical flow reactor (see Note S8 and Figure S10 for details) and shipped
to Shanghai, China. For this experiment, 5 mg of CoPc@C was loaded inside the
Figure 5. MOST to power generation performance
(A) Schematic concept of MOST to power generation.
(B) NBD couple-based solar energy storage for power-generation experimental setup.
(C) Heat release monitoring by thermocouple and voltage generated from MEMS-TEG chip over
time. The inset is a photo of the device. Scale bar, 1 cm.
(D) Schematic experimental setup of AZO film-based solar energy for power generation.
(E) Net voltage generated from MEMS-TEG chip over time. The inset is a photo of the device. Scale
bar, 1 cm.
8 Cell Reports Physical Science 3, 100789, March 16, 2022
catalytic reactor (inside the central copper tube), where a thermally conductive pad
was used to fill the gap between copper plates in the device (see Figure 5B). The
reactor was placed above the MEMS-TEG chip, and the whole setup was then placed
on top of an aluminum brick heat sink, which ensured a stable ambient temperature
and served as the cold side of the device. Importantly, the hot side of the system was
covered with thermally insulated plastic foam to ensure that the heat generated was
reflected instead of being lost to the environment. As a result, with less than 1 mL of a
0.78 M solution and a flow speed of 5 mL h 1
, a measured bias voltage of up to
0.18 mV was recorded. According to the MEMS-TEG chip characterization, this
voltage can generate a maximum power output of z0.1 nW (power output density
of 1.3 W m 3
, see Figure 5C). With the same flow speed, a continuous operating test
with slightly lower concentration of 0.62 M in toluene was also performed. This suc-
cessfully generated, for the first time, a total electric energy of up to 0.44 W h$m 3
over 24 min (see Note S9 and Figure S11).
In the case of AZO, a smaller amount of material was used; 7 mg of cis-AZO, gener-
ated from a 365 nm LED light source, was loaded onto the thermally conductive pad.
A polyethylene terephthalate (PET) film was gently pressed on top of the material to
allow it to fully cover the surface of the MEMS-TEG chip evenly. Laser irradiation at
532 nm triggered the back conversion (see Figure 5D), leading to a bias output
voltage of up to 0.13 mV. This corresponds to a maximum power output of 0.06
nW (power output density of 0.7 W m 3
) (see Note S10 and Figures S12–S15 for de-
tails). Interestingly, various peaks were observed when the voltage approached the
maximum. This was likely due to the complex release of heat, which involved both
photoisomerization and phase transitions (see Figure 5E). We observed that less po-
wer is generated from cis-AZO than from QC, although the former reached a higher
surface temperature, but the temperature distribution in the latter tube is more
even. Not surprisingly, this is because the amount of heat released from these two
systems is markedly different: 1 mL of 0.78 M QC could produce 72.5 J, while
7 mg of cis-AZO could produce only 2.3 J of energy.
Here, we noticed that the maximum temperatures reached by the NBD couple and
the AZO couple are 37
C and 52
C, respectively, while the corresponding voltages
generated by MEMS-TEG are 0.18 and 0.13 mV, respectively. However, compared
with the hot water with similar temperature, the maximum power output density
generated by the NBD couple and the AZO couple is greatly reduced. It is worth
noting that the hot water flowing continuously and rapidly in the copper reactor
has a better thermal contact surface with the pipe wall than the discharging QC so-
lution and cis-AZO film. Consequently, the hot water flowing at a temperature of
C makes the power density generated by MEMS-TEG nearly 5 times that of
the QC solution with similar temperature (37
C). This demonstrates that, with the
MOST materials at hand, better thermal management and TE materials may increase
the power output of the next generation of devices.
To the best of our knowledge, these results show the first proof of principle that so-
lution-based MOST and PCM-MOST systems can generate electric power. Future
work should focus on red shifting the absorption band (capturing more sunlight)
and increasing the temperature gradient produced by the back reaction (improving
energy density). The next generation of combined devices should include a better
thermal management system to avoid heat dissipation from the MOST system to
the surrounding environment, thereby increasing the amount of heat energy con-
verted to electrical power output. Based on the TE film preparation method,60
TE efficiency can be simulated to be over 8% at room temperature (ZTave = 2.4)
Cell Reports Physical Science 3, 100789, March 16, 2022 9
and around 29% between 0 and 100 K (ZTave = 1.0) with a temperature difference of
C (see Note S11 and Figure S16 for details), assuming that MOST systems can
achieve this absolute temperature of 100
C, which is close to what has recently been
Producing a highly soluble photoswitch of ca. 1.5 M, accompanied
by a heat release of 100 kJ mol 1
with a 5 mL h 1
flow speed, would allow the system
to produce a power output of 16.7 mW (0.2 GW m 3
) at room temperature and 60.4
mW (0.7 GW m 3
) at temperatures of 0–100 K. This would be enough to power a low-
power-supplied Internet of Things device on Earth or in the outer space
In this work, we have shown two molecular photoswitches in different physical forms
(liquid-based NBD and neat AZO film) for coupling MOST systems with electrical po-
wer generation via MEMS-TEG devices. The liquid-based NBD exhibits a solar en-
ergy storage efficiency of z0.5% in 0.5 mM toluene, which is more efficient than
NBD was also, for the first time, tested through 54
charge and discharge cycles in a continuously operating energy storage and
catalyzed release cycle, and showed no sign of degradation. Alternatively, the
PCM-MOST hybrid neat AZO film captures and releases energy in photochemical
solid-liquid transitions, which allows the MOST system to harness energy both
from sunlight and from the ambient environment, meaning that upgraded heat
can be produced on demand. Comparing the two candidates, both of them can
store solar energy in the visible range for over a month at room temperature. To
improve the macroscopic heat-release capability, future investigation of increasing
the solubility of liquid-based NBD is necessary. For neat AZO, with addition phase-
change properties, the overall energy storage capacity has been greatly improved.
However, due to the light-induced back-conversion property of AZO, for future real-
world-conditions device design, it is necessary to add a band-pass filter that is able
to filter out the photons that initiate back conversion of AZO.
To demonstrate generation of power from the MOST system, an ultrathin-film-
based, highly sensitive MEMS-TEG device was used to capture the heat released
from either scenario. For the first time, electricity was produced in this setup, with
power output up to 0.1 nW (power output per unit volume up to 1.3 W m 3
more, this device continuously generated electricity, for the first time, for over
25 min. We note that this is a very compact and local solar energy storage-power
generation system that operates through a mechanism entirely different from tradi-
tional PV-battery storage combinations. Furthermore, these systems can be charged
and discharged across different geographic locations (Sweden to China in this work)
over a few months, showing that solar energy can be stored for power generation on
demand. Although the efficiency of these systems needs to be improved, we envi-
sion that they can be used in local power generation applications in the future.
Further information and requests for resources and procedures should be directed to
the lead contact, Prof. Kasper Moth-Poulsen (email@example.com).
NBD and AZO were synthesized by following the existing procedure in the litera-
All QC samples were prepared by irradiating an NBD solution with a
340 nm LED light source from Thorlabs. The conversion percentage was checked
by either a 1
H NMR 400 MHz instrument or a Cary 60 UV-vis spectrophotometer.
10 Cell Reports Physical Science 3, 100789, March 16, 2022
CoPc@C catalyst was produced by following the existing procedure.3
state was prepared using a 365 nm LED light source. For photoinduced back conver-
sion, a 532 nm laser (110 mW cm 2
, the beam diameter of 1.3 cm) was used to
prepare the trans-AZO state by irradiating the cis-AZO sample. All solution-based
spectroscopic measurements were performed in a cuvette with path length of
1 cm on a Cary 100 UV-vis spectrophotometer, scanning the wavelength from 750
to 290 nm. Absorption spectra for the outdoor test were recorded by two microflow
cells and a portable spectrometer, which was purchased from Avantes. Teflon plastic
tubing used was from Cole-Parmer Instrument Company.
Data and code availability
All of the data supporting the findings are presented within the article and supple-
mental information. All other data are available from the lead contact upon reason-
Supplemental information can be found online at https://doi.org/10.1016/j.xcrp.
This work was supported by the K. A. Wallenberg Foundation, the Swedish Foun-
dation for Strategic Research, the Swedish Research Council Formas, the Swedish
Energy Agency, the European Research Council (ERC) under grant agreement
CoG, PHOTHERM - 101002131, the Catalan Institute of Advanced Studies (ICREA),
and the European Union’s Horizon 2020 Framework Programme under grant agree-
ment no. 951801. The MEMS-TEG chip manufacture and experimentation were sup-
ported by the National Natural Science Foundation of China (grant 51776126). The
authors would like to thank the Center for Advanced Electronic Materials and De-
vices (AEMD) and Instrumental Analysis Center of Shanghai Jiao Tong University
(SJTU) and the startup fund of Shanghai Jiao Tong University. We thank Dr. Sarah
Lerch and Prof. Ben Greatrex for reading and commenting on the manuscript. We
acknowledge Neuroncollective.com and Daniel Spacek for the graphical abstract.
Z. Wang performed all the material and MEMS-TEG chip characterizations, conver-
sion tests, cycling tests, heat-release experiments, and power-generation demon-
strations. Z. Wu carried out the MEMS-TEG chip fabrication, characterization, and
TE efficiency simulation. E.M. and Z.Y.Z. performed the heat-release experiments
and power-generation experiments. Y.L., X.F., and F.W. performed MEMS-TEG
chip fabrication. J.O.H. performed the sample preparation with an automated
flow system. M.J. and Z.Y.Z. synthesized the used compounds. Z. Wang, Z.H.,
T.L., and K.M.P. designed the experiments. All authors contributed to writing the
DECLARATION OF INTERESTS
The authors declare no competing interests.
Received: November 15, 2021
Revised: January 26, 2022
Accepted: February 7, 2022
Published: March 2, 2022
Cell Reports Physical Science 3, 100789, March 16, 2022 11
1. Masson-Delmotte, V., Zhai, P., Pörtner, H.O.,
Roberts, D., Skea, J., and Shukla, P.R. (2019).
Global warming of 1.5
C (IPCC). https://www.
2. BP plc (2019). BP statistical review of world
energy, 68 edition. https://www.bp.com/
3. Gautam, P., Kumar, S., and Lokhandwala, S.
(2019). Chapter 11 - energy-aware intelligence
in megacities. In Current Developments in
Biotechnology and Bioengineering, S. Kumar,
R. Kumar, and A. Pandey, eds. (Elsevier),
pp. 211–238. https://doi.org/10.1016/B978-0-
4. Parsons, J., Buongiorno, J., Corradini, M., and
Petti, D. (2019). A fresh look at nuclear energy.
Science 363, 105. https://doi.org/10.1126/
5. Lewis, N.S., and Nocera, D.G. (2006). Powering
the planet: chemical challenges in solar energy
utilization. Proc. Natl. Acad. Sci. U S A 103,
6. Perez, R., and Perez, M. (2015). IEA-SHCP-
Newsletter 62, https://research.asrc.albany.
7. Perez, R., and Perez, M. (2009). IEA-SHCP-
Newsletter 50, https://www.iea-shc.org/data/
8. Kandeal, A.W., Thakur, A.K., Elkadeem, M.R.,
Elmorshedy, M.F., Ullah, Z., Sathyamurthy, R.,
and Sharshir, S.W. (2020). Photovoltaics
performance improvement using different
cooling methodologies: a state-of-art review.
J. Clean. Prod. 273, 122772. https://doi.org/10.
9. Martinho, F. (2021). Challenges for the future of
tandem photovoltaics on the path to terawatt
levels: a technology review. Energy Environ.
Sci. 14, 3840–3871. https://doi.org/10.1039/
10. Asefi, G., Habibollahzade, A., Ma, T., Houshfar,
E., and Wang, R.Z. (2021). Thermal
management of building-integrated
photovoltaic/thermal systems: a
comprehensive review. Sol. Energy 216,
11. Sobri, S., Koohi-Kamali, S., and Rahim, N.A.
(2018). Solar photovoltaic generation
forecasting methods: a review. Energy
Convers. Manag. 156, 459–497. https://doi.
12. Herrmann, U., Kelly, B., and Price, H. (2004).
Two-tank molten salt storage for parabolic
trough solar power plants. Energy 29,
13. Du, K., Calautit, J., Wang, Z., Wu, Y., and Liu, H.
(2018). A review of the applications of phase
change materials in cooling, heating and
power generation in different temperature
ranges. Appl. Energy 220, 242–273. https://doi.
14. Xiong, Y., Zhang, L., Weis, P., Naumov, P., and
Wu, S. (2018). A solar actuator based on
hydrogen-bonded azopolymers for electricity
generation. J. Mater. Chem. A 6, 3361–3366.
15. Yoshida, Z.-i. (1985). New molecular energy
storage systems. J. Photochem. 29, 27–40.
16. Moth-Poulsen, K.,
Coso, D., Börjesson, K.,
Vinokurov, N., Meier, S.K., Majumdar, A.,
Vollhardt, K.P.C., and Segalman, R.A. (2012).
Molecular solar thermal (MOST) energy
storage and release system. Energy Environ.
Sci. 5, 8534–8537. https://doi.org/10.1039/
17. Kolpak, A.M., and Grossman, J.C. (2011).
Azobenzene-functionalized carbon nanotubes
as high-energy density solar thermal fuels.
Nano Lett. 11, 3156–3162. https://doi.org/10.
18. Kucharski, T.J., Ferralis, N., Kolpak, A.M.,
Zheng, J.O., Nocera, D.G., and Grossman, J.C.
(2014). Templated assembly of photoswitches
significantly increases the energy-storage
capacity of solar thermal fuels. Nat. Chem. 6,
19. Bren, V.A., Dubonosov, A.D., Minkin, V.I., and
Chernoivanov, V.A. (1991). Norbornadiene–
quadricyclane—an effective molecular system
for the storage of solar energy. Russ. Chem.
Rev. 60, 451–469. https://doi.org/10.1070/
20. Broman, S., Brand, S., Parker, C., Petersen, M.,
Tortzen, C., Kadziola, A., Kilså, K., and Nielsen,
M. (2011). Optimized synthesis and detailed
NMR spectroscopic characterization of the
photoswitch. Arkivoc 2011, 51–67. https://doi.
21. Wang, Z., Roffey, A., Losantos, R., Lennartson,
A., Jevric, M., Petersen, A.U., Quant, M., Dreos,
A., Wen, X., Sampedro, D., et al. (2019).
Macroscopic heat release in a molecular solar
thermal energy storage system. Energy
Environ. Sci. 12, 187–193. https://doi.org/10.
22. Cacciarini, M., Vlasceanu, A., Jevric, M., and
Nielsen, M. (2017). An effective trigger for
energy release of vinylheptafulvene-based
solar heat batteries. Chem. Commun. 53.
23. Brummel, O., Waidhas, F., Bauer, U., Wu, Y.,
Bochmann, S., Steinrück, H.-P., Papp, C.,
Bachmann, J., and Libuda, J. (2017).
Photochemical energy storage and
electrochemically triggered energy release in
the norbornadiene–quadricyclane system: UV
photochemistry and IR
spectroelectrochemistry in a combined
experiment. J. Phys. Chem. Lett. 8, 2819–2825.
24. Waidhas, F., Jevric, M., Bosch, M., Yang, T.,
Franz, E., Liu, Z., Bachmann, J., Moth-Poulsen,
K., Brummel, O., and Libuda, J. (2020).
Electrochemically controlled energy release
from a norbornadiene-based solar thermal
fuel: increasing the reversibility to 99.8% using
Hopg as the electrode material. J. Mater.
Chem. A 8, 15658–15664. https://doi.org/10.
25. Fu, L., Yang, J., Dong, L., Yu, H., Yan, Q., Zhao,
F., Zhai, F., Xu, Y., Dang, Y., Hu, W., et al. (2019).
Solar thermal storage and room-temperature
fast release using a uniform flexible
azobenzene-grafted polynorborene film
enhanced by stretching. Macromolecules 52,
26. Hu, J., Huang, S., Yu, M., and Yu, H. (2019).
Flexible solar thermal fuel devices: composites
of fabric and a photoliquefiable azobenzene
derivative. Adv. Energy Mater. 9, 1901363.
27. Yan, Q., Zhang, Y., Dang, Y., Feng, Y., and
Feng, W. (2020). Solid-state high-power photo
heat output of 4-((3,5-dimethoxyaniline)-
diazenyl)-2- imidazole/graphene film for
thermally controllable dual data encoding/
reading. Energy Storage Mater. 24, 662–669.
28. Wang, Z., Moı̈se, H., Cacciarini, M., Nielsen,
M.B., Morikawa, M.-a., Kimizuka, N., and Moth-
Poulsen, K. (2021). Liquid-based multijunction
molecular solar thermal energy collection
device. Adv. Sci. 8, 2103060. https://doi.org/10.
29. Jaziri, N., Boughamoura, A., Müller, J.,
Mezghani, B., Tounsi, F., and Ismail, M. (2020).
A comprehensive review of thermoelectric
generators: technologies and common
applications. Energy Rep. 6, 264–287. https://
30. Shi, X.-L., Zou, J., and Chen, Z.-G. (2020).
Advanced thermoelectric design: from
materials and structures to devices. Chem. Rev.
120, 7399–7515. https://doi.org/10.1021/acs.
31. Wu, Z., Zhang, S., Liu, Z., Mu, E., and Hu, Z.
(2022). Thermoelectric converter: strategies
from materials to device application. Nano
Energy 91, 106692. https://doi.org/10.1016/j.
32. Weinstein, L.A., Loomis, J., Bhatia, B., Bierman,
D.M., Wang, E.N., and Chen, G. (2015).
Concentrating solar power. Chem. Rev. 115,
33. Kraemer, D., Jie, Q., McEnaney, K., Cao, F., Liu,
W., Weinstein, L.A., Loomis, J., Ren, Z., and
Chen, G. (2016). Concentrating solar
thermoelectric generators with a peak
efficiency of 7.4%. Nat. Energy 1, 16153.
34. Li, G., Fernández, J.G., Ramos, D.A.L., Barati,
V., Pérez, N., Soldatov, I., Reith, H., Schierning,
G., and Nielsch, K. (2018). Integrated
microthermoelectric coolers with rapid
12 Cell Reports Physical Science 3, 100789, March 16, 2022
response time and high device reliability. Nat.
Electron. 1, 555–561. https://doi.org/10.1038/
35. Mu, E., Wu, Z., Wu, Z., Chen, X., Liu, Y., Fu, X.,
and Hu, Z. (2019). A novel self-powering
ultrathin TEG device based on micro/nano
emitter for radiative cooling. Nano Energy 55,
36. Mu, E., Yang, G., Fu, X., Wang, F., and Hu, Z.
(2018). Fabrication and characterization of
ultrathin thermoelectric device for energy
conversion. J. Power Sources 394, 17–25.
37. Liu, Y., Mu, E., Wu, Z., Che, Z., Sun, F., Fu, X.,
Wang, F., Wang, X., and Hu, Z. (2020). Ultrathin
MEMS thermoelectric generator with Bi2Te3/
(Pt, Au) multilayers and Sb2Te3 legs. Nano
Converg. 7, 8. https://doi.org/10.1186/s40580-
38. Jevric, M., Petersen, A.U., Mansø, M., Kumar
Singh, S., Wang, Z., Dreos, A., Sumby, C.,
Nielsen, M.B., Börjesson, K., Erhart, P., and
Moth-Poulsen, K. (2018). Norbornadiene-
based photoswitches with exceptional
combination of solar spectrum match and
long-term energy storage. Chem. Eur. J. 24,
39. Dreos, A., Wang, Z., Udmark, J., Ström, A.,
Erhart, P., Börjesson, K., Nielsen, M.B., and
Moth-Poulsen, K. (2018). Liquid norbornadiene
photoswitches for solar energy storage. Adv.
Energy Mater. 8, 1703401. https://doi.org/10.
40. Wang, Z., Losantos, R., Sampedro, D.,
Morikawa, M.-a., Börjesson, K., Kimizuka, N.,
and Moth-Poulsen, K. (2019). Demonstration of
an azobenzene derivative based solar thermal
energy storage system. J. Mater. Chem. A 7,
41. Masutani, K., Morikawa, M.-a., and Kimizuka, N.
(2014). A liquid azobenzene derivative as a
solvent-free solar thermal fuel. Chem.
Commun. 50, 15803–15806. https://doi.org/10.
42. Quant, M., Lennartson, A., Dreos, A., Kuisma,
M., Erhart, P., Börjesson, K., and Moth-Poulsen,
K. (2016). Low molecular weight norbornadiene
derivatives for molecular solar-thermal energy
storage. Chem. Eur. J. 22, 13265–13274.
43. Petersen, A.U., Hofmann, A.I., Fillols, M.,
Mansø, M., Jevric, M., Wang, Z., Sumby, C.J.,
Müller, C., and Moth-Poulsen, K. (2019). Solar
energy storage by molecular norbornadiene–
quadricyclane photoswitches: polymer film
devices. Adv. Sci. 6, 1900367. https://doi.org/
44. Morikawa, M.-a., Yang, H., Ishiba, K., Masutani,
K., Hui, J.K.-H., and Kimizuka, N. (2020). A liquid
arylazopyrazole derivative as molecular solar
thermal fuel with long-term thermal stability.
Chem. Lett. 49, 736–740. https://doi.org/10.
45. Wang, Z., Udmark, J., Börjesson, K., Rodrigues,
R., Roffey, A., Abrahamsson, M., Nielsen, M.B.,
and Moth-Poulsen, K. (2017). Evaluating
photoswitches for solar energy storage
applications. ChemSusChem 10, 3049–3055.
46. Zhang, Z.-Y., He, Y., Wang, Z., Xu, J., Xie, M.,
Tao, P., Ji, D., Moth-Poulsen, K., and Li, T.
(2020). Photochemical phase transitions enable
coharvesting of photon energy and ambient
heat for energetic molecular solar thermal
batteries that upgrade thermal energy. J. Am.
Chem. Soc. 142, 12256–12264. https://doi.org/
47. Zhang, Z.-Y., He, Y., Zhou, Y., Yu, C., Han, L.,
and Li, T. (2019). Pyrazolylazophenyl ether-
based photoswitches: facile synthesis, (near-)
quantitative photoconversion, long thermal
half-life, easy functionalization, and versatile
applications in light-responsive systems.
Chem. Eur. J. 25, 13402–13410. https://doi.org/
48. Shi, Y., Gerkman, M.A., Qiu, Q., Zhang, S., and
Han, G.G.D. (2021). Sunlight-activated phase
change materials for controlled heat storage
and triggered release. J. Mater. Chem. A.
49. Gerkman, M.A., and Han, G.G.D. (2020).
Toward controlled thermal energy storage and
release in organic phase change materials.
50. Gerkman, M.A., Gibson, R.S.L., Calbo, J., Shi,
Y., Fuchter, M.J., and Han, G.G.D. (2020).
Arylazopyrazoles for long-term thermal energy
storage and optically triggered heat release
C. J. Am. Chem. Soc. 142, 8688–8695.
51. Han, G.G.D., Li, H., and Grossman, J.C. (2017).
Optically-controlled long-term storage and
release of thermal energy in phase-change
materials. Nat. Commun. 8, 1446. https://doi.
52. Ishiba, K., Morikawa, M.-a., Chikara, C.,
Yamada, T., Iwase, K., Kawakita, M., and
Kimizuka, N. (2015). Photoliquefiable ionic
crystals: a phase crossover approach for
photon energy storage materials with
functional multiplicity. Angew. Chem. Int. Ed.
Engl. 54, 1532–1536. https://doi.org/10.1002/
53. Xu, X., Wu, B., Zhang, P., Xing, Y., Shi, K., Fang,
W., Yu, H., and Wang, G. (2021).
Arylazopyrazole-based dendrimer solar
thermal fuels: stable visible light storage and
controllable heat release. ACS Appl. Mater.
Interfaces 13, 22655–22663. https://doi.org/10.
54. Xu, X., Zhang, P., Wu, B., Xing, Y., Shi, K., Fang,
W., Yu, H., and Wang, G. (2020). Photochromic
dendrimers for photoswitched solid-to-liquid
transitions and solar thermal fuels. ACS Appl.
Mater. Interfaces 12, 50135–50142. https://doi.
55. Cai, F., Song, T., Yang, B., Lv, X., Zhang, L., and
Yu, H. (2021). Enhancement of solar thermal
fuel by microphase separation and
nanoconfinement of a block copolymer. Chem.
Mater. 33, 9750–9759. https://doi.org/10.1021/
56. Hansen, M.H., Olsen, S.T., Sylvester-Hvid, K.O.,
and Mikkelsen, K.V. (2019). Simulation
framework for screening of molecular solar
thermal systems in the context of a hybrid
device. Chem. Phys. 519, 92–100. https://doi.
57. Dresselhaus, M.S., Dresselhaus, G., Sun, X.,
Zhang, Z., Cronin, S.B., and Koga, T. (1999).
Low-dimensional thermoelectric materials.
Phys. Solid State 41, 679–682. https://doi.org/
58. Latorre-Pérez, A., Vilanova, C., Alcaina, J.J.,
and Porcar, M. (2019). Thermoelectric heat
exchange and growth regulation in a
continuous yeast culture. Microbiologyopen 8,
59. Han, C.-G., Qian, X., Li, Q., Deng, B., Zhu, Y.,
Han, Z., Zhang, W., Wang, W., Feng, S.-P.,
Chen, G., and Liu, W. (2020). Giant
thermopower of ionic gelatin near room
temperature. Science 368, 1091–1098. https://
60. Venkatasubramanian, R., Siivola, E., Colpitts,
T., and O’Quinn, B. (2001). Thin-film
thermoelectric devices with high room-
temperature figures of merit. Nature 413,
61. Lee, H.G., and Chang, N. (2015). Powering the
IoT: storage-less and converter-less energy
harvesting. In The 20th Asia and South Pacific
Design Automation Conference, 19-22 (IEEE),
pp. 124–129. https://doi.org/10.1109/
62. Scharf, H.-D., Fleischhauer, J., Leismann, H.,
Ressler, I., Schleker, W.-g., and Weitz, R. (1979).
Criteria for the efficiency, stability, and capacity
of abiotic photochemical solar energy storage
systems. Angew. Chem. Int. Ed. Engl. 18,
Cell Reports Physical Science 3, 100789, March 16, 2022 13